Sulfuric Acid Assisted Preparation of Red-Emitting Carbonized Polymer Dots and the Application of Bio-Imaging
Nanoscale Research Letters
December 2018, 13:272 | Cite as
Sulfuric Acid Assisted Preparation of Red-Emitting Carbonized Polymer Dots and the Application of Bio-Imaging
AuthorsAuthors and affiliations
Chunlin TanChao ZhouXingyun PengHuozhen ZhiDan WangQiuqiang ZhanSailing He
First Online: 10 September 2018
Received: 22 March 2018
Accepted: 06 August 2018
Part of the following topical collections:Low Dimensional Electric and Photonic Materials and Devices
Red-emitting carbonized polymer dots (CPDs) was prepared from p-phenylenediamine (p-PD) aqueous solution with the assistance of sulfuric acid (H2SO4), and the optical properties and bio-imaging application were studied in this paper. Compared with other strong acids-assisted systems, SA-CPDs (prepared from H2SO4-assisted system, average diameter is ~ 5 nm) is the brightest. The photoluminescence Quantum Yields (QYs) is 21.4% (in water), and the product yield is 16.5%. SA-CPDs aqueous solution emits at 600 nm when excited by the light from 300 to 580 nm. The emission wavelength is independent on the excitation wavelength. Formation energies of CPDs in two ways were calculated to show that longitudinal growth (forming polymers) is difficult, and the transverse growth (forming CPDs) is easy. In addition, the two-photon photoluminescence properties (emitting at 602 nm when excited by 850 nm femtosecond pulse laser) of SA-CPDs were also utilized in the experiments for HeLa cells staining and shown to have potential applications in bio-imaging.
KeywordsCarbon dots Carbonized polymer dots Red-emitting Fluorescence Sulfuric acid assisted Hydrothermal
Carbonized polymer dots
Carbon Dots were prepared from p-PD with HCl-assisted system
Carbon Dots were prepared from p-PD with HClO4-assisted system
Carbon Dots were prepared from p-PD with H2SO4-assisted system
Electronic supplementary material
The online version of this article ( https://doi.org/10.1186/s11671-018-2657-4) contains supplementary material, which is available to authorized users.
Carbon dots (CDs) have attracted much attention due to their advantages including excellent water solubility, optical stability, unique fluorescence properties, low toxicity, low cost, etc . Most CDs were studied as potential candidates for various applications, such as electrochemical immune-sensors , bio-imaging [3, 4, 5, 6] sensors [7, 8, 9, 10, 11, 12], photo-catalysis [13, 14, 15], light-emitting devices , and optoelectronics [17, 18, 19]. Synthesis of CDs plays an important role in the studies on the optical properties and applications. The reported approaches to prepare CDs could be mainly summarized as the “top-down” from various carbon materials and “bottom-up” from organic molecules, polymers, or natural products . The “bottom-up” methods are efficient routes for the synthesis of fluorescent CDs in large scale . Groups in the applied molecules including –OH, –COOH, –C=O, and –NH2 can be dehydrated and carbonized in elevated temperature by hydrothermal, microwave, combustion, pyrolysis, and so on.
Red-emitting dots have aroused considerable interests because of, i.e., the larger penetration depth in bio-imaging field. Especially, the pure color dots are critical to a certain occasion because the excitation-wavelength-independent luminescence materials can provide a single and stable photoluminescence (PL) light. Most emissions of CDs are excitation-wavelength-dependent, and CDs usually emit blue, green, or yellow light, few CDs emit bright red light .
Recently, isomers of phenylenediamine (PD), such as o-, m-, and p-PD, had been studied as carbon sources to prepare CDs [8, 9, 23, 24]. Blue-, green-, and red-emitting CDs can be prepared from m-, o-, and p-PD ethanol solution, respectively . Full-color light-emitting CDs can be prepared from p-PD and urea aqueous solution . In our previous work , we proposed that new red carbon dots (Quantum yields = 15.8%, in water) can be synthesized facilely from “p-PD + HNO3” aqueous system and applied in the detection of metal ions in water. Recently, the similar “o-PD + H3PO4”  and “o-PD + HNO3”  systems were reported, and Liu et al.  renamed their CDs (QYs = 10.8%, in water) as “carbonized polymer dots (CPDs).” Unlike the traditional carbon dots, the CPDs’ emission wavelengths do not depend on the excitation wavelength, and thus the PD-based “CDs” should be named more accurately as CPDs.
Herein, we report a facile and high-efficient method of strong acid-assisted hydrothermal route to prepare red-emitting CPDs and the application of bio-imaging with two-photon photoluminescence properties. Mechanism for the formation of CPDs is proposed by using Gaussian 09 program package.
Synthesis of Red CPDs From Acid-Assisted p-PD Systems
Based on our previous work , we selected sulfuric acid (H2SO4), hydrochloric acid (HCl), and perchloric acid (HClO4) as the assistants for the preparation of red CPDs, the corresponding CPDs were labeled as SA-CPDs, HC-CPDs, and PA-CPDs, respectively. In order to optimize the experimental conditions of H2SO4-assisted system, we selected several parameters, such as c (acid) to c (p-PD) ratio, c (p-PD), temperature (T), and reaction time (t). CPDs products were washed by hexane to remove the unreacted p-PD and by ethyl alcohol to remove acids, centrifuged at 14000 rpm for 30 min to remove polymer precipitation, and filtered through a 0.22 μm filter membrane. If powder is desirable, the purified CPDs solution can be further evaporated by rotary evaporator to near dry state at 80 °C and a low vacuum condition (the remaining will be of powder form).
Characterization and Measurement
High-resolution TEM (HR-TEM) images were recorded on JEM-2100 transmission microscope operating at 200 kV. Infrared spectra of CPDs solutions were collected using Prestige-21 FT-IR spectrometer by use of KRS-5 window slices (mixture of TlBr and TlI), typically, liquid phases were dropped on one slice and dried. The slice was covered by the other slice and fixed on the testing stand. Then the infrared spectra were recorded.
The fluorescence spectra of CPDs were measured on F-2500 fluorescence spectrophotometer. UV-Vis absorption spectra were recorded on Lambda 950 UV/VIS/NIR Spectrometer. The two-photon emission spectra of CPDs were recorded by a fiber spectrograph (QE65000, Ocean Optics) in the microscope system. SA-CPDs aqueous solution and the powders re-dissolved solution were spun on slides, and the two-photon photoluminescence properties were then measured.
Photoluminescence quantum yields (QYs) of the CPDs were measured with Rhodamine B (QYs = 56% in ethanol) as the reference dye at the emission range of 580–610 nm excited by 365 nm UV light [25, 28], the procedure of QYs measurements were shown in the Additional file 1.
The Gaussian 09 package was used for the density function theory (DFT) calculations . The equilibrium structures were optimized by B3LYP method in conjunction with the 6–311++G (d) basis set level . To investigate the role of solvent effects, water was utilized in polarized continuum model (PCM). Frequency analyses were done with the same level for confirming that each optimized structure corresponded to a stationary point.
Cell Culture and Treatment
1.35 mL of HeLa cells in Dulbecco’s Modified Eagle Medium (DMEM; Gibco) at an initial density of 4 × 104 cell per milliliters were seeded in each dish and cultured at 37 °C for 24 h under a humidified atmosphere containing 5% CO2. SA-CPDs powders were re-dissolved in water to prepare the reserve solution (400 μg mL− 1). 1350 μL cells were cultured with 150 μL SA-CPDs reserve solution (the final concentration is 40 μg mL− 1) for 12 h and then washed three times with PBS to remove the free SA-CPDs. Finally, the cellular imaging results were collected with a confocal microscope under 850-nm femtosecond laser excitation (30 mW).
Results and Discussion
Optimizing Preparation for Red CPDs
In basic experiments, different acid-assisted systems with various concentration ratios, reaction temperatures, and times were investigated (see Additional file 1: Figure S1). We found that red CPDs can be formed above 180 °C (reacting for 2 h) for different acids systems, and the reactions are not affected by anions in the solutions. Long-time (4–12 h, 240 °C for H3PO4 and HF systems, see Additional file 1: Figure S1f) reaction will increase the particle size, and the red fluorescence will be eventually faded, while the fluorescence change is not obvious for HCl system (2–6 h, 200 °C, see Additional file 1: Figure S2). Considering the energy saving and upper temperature limit of Teflon liner, optimum temperature and reaction time are selected as 200 °C and 2 h respectively. Based on the optimization strategy of p-PD + HCl system (see Additional file 1: Figure S2), we optimized the p-PD + H2SO4 and p-PD + HClO4 systems and obtained the optimization results shown as Table 1.
The selected experimental parameters of p-PD + acids systems
c (p-PD) (M)
c (acid) (M)
p-PD + H2SO4
p-PD + HCl
p-PD + HClO4
SA-CPDs, HC-CPDs, and PA-CPDs were prepared from p-PD solution with the assistance of H2SO4, HCl, and HClO4, respectively. The optimized c (acid) to c (p-PD) ratios of H2SO4-, HCl-, and HClO4-assisted systems are 1, 3, and 3, respectively (see Additional file 1: Figure S3a). The suitable c (p-PD) range for the preparation of red CPDs is wide (from 0.02 to 0.20 mol L− 1). The optimized temperature (T) and the reaction time (t) are 200 °C and 2 h. SA-CPDs is the brightest red CPDs with a high QYs of 21.4% (Additional file 1: Figure S3b). There are two reasons why H2SO4-assisted carbon dots have a better quality compared to HCl-, HClO4-, and HNO3-assisted ones (published in our previous work ). First, H2SO4 is a non-volatile strong acid which maintains its acidity in a high temperature and high pressure reaction solution. Second, H2SO4-assisted system is the only one that can form ammonium salt precipitation in precursor, and the precipitates release the free reactants slowly, avoiding the formation of large particle polymer precipitation and further promoting the formation of high quality carbon dots. HA-CPDs and PA-CPDs are dark-red-brown thick solutions and emit dark red PL under 365 nm UV light irradiation, while the as-prepared SA-CPDs is bright-red transparent thin solution and emits bright red light (Additional file 1: Figure S3c). After being purified by washing, concentration, filtering, and evaporation, dark-red-brown powders of SA-CPDs (Additional file 1: Figure S3d) were obtained with the product yield of 16.5%. The powders can be re-dissolved in water and the solution emits bright and red fluorescence (Additional file 1: Figure S3e).
TEM characterization and FT-IR analysis
TEM images of sample OpPD (without H2SO4 ) and SA-CPDs (with H2SO4) were shown in Fig. 1. Sample OpPD is composed of fragments (oligomers, Fig. 1a) and polymers (Fig. 1a insert). SA-CPDs are monodispersed CPDs with the average size of ~ 5 nm (Fig. 1c). It exhibits well-resolved lattice fingers with a space of ~ 0.21 nm (Fig. 1b insert), corresponding to the (100) in-plane lattice spacing of graphene [31, 32].
Open image in new window
TEM images of sample OpPD (without H2SO4) (a) and SA-CPDs (b). c The size distribution of SA-CPDs. d The FT-IR spectra of sample OpPD and red CPDs. Sample OpPD and SA-CPDs were prepared from p-PD aqueous solution without and with H2SO4-assisted
Surface states of CPDs may affect the optical properties. The surface chemical groups of sample OpPD and SA-CPDs were characterized by FT-IR spectra (Fig. 1d). Two samples have several similar groups, such as Ar-H (2700–3200 cm− 1 , belongs to aromatic C-H stretching vibration), C-C (~ 1433 cm− 1, belongs to aromatic C-bone stretching vibration, reveals the presence of aromatic stretching vibrations characteristic to benzenoid units) , and C=O (1628 cm− 1, belongs to the –COOH groups). Compared with sample OpPD, the new groups, such as O-H (3300–3700 cm− 1 and 1175 cm− 1 belong to the –COOH groups), C-O-C (1055 cm− 1, exist in esters), and C-H (2400–3000 cm− 1 belongs to alkyl radicals formed in ring-opening reaction), are found in the CPDs, while the –NH2 or –NH– related groups such as N-H (3100–3300 cm− 1 and 1512 cm− 1 and C-N (1126, 1261, and 1305 cm− 1 belong to the free –NH2 or –NH– groups from p-PD precursor, are weaken or disappeared. The existence of –OH or –COOH groups indicates that the oxidation degree of the surface of SA-CPDs (with H2SO4 adding) is higher than that of sample OpPD (without acid addition).
Proposed Mechanism for the Formation of CDs
Formation energies were calculated using the Gaussian 09 program package. After being protonated by acid-assisting, bi-polymers may be polymerized in two ways that called longitudinal and transverse growth. The calculated formation energy of transverse growth (− 1406.07 kJ mol− 1) is significantly higher than that of longitudinal growth (− 616.25 kJ mol− 1). It shows that the fully protonated bi-polymers (pH 3, after excess H+ was added) tend to be polymerized in transverse way to form planar structure (Fig. 2). These planar structures were then self-assembled to form spherical CPDs.
Open image in new window
Formation energies of longitudinal and transverse growths
Although being prepared by the assistance of different acids, all CPDs have the similar optical properties . For the UV-Vis spectra of SA-CPDs aqueous solution (Fig. 3a), the absorbance peak located at ~ 290 nm is associated to the transitions in benzene ring, and the peaks located at 430 nm and 510 nm could be assigned to π-π* transition of substituted phenazine conjugated to the lone electron pairs on the adjacent amine group and the electron transition from the benzenoid ring to the quinoid rings, respectively . The excitation curve describes a wide and a gradual upward trend at visible region, and the maximum excitation peak (~ 580 nm) is close to the emission peak (~ 600 nm). The CPDs emit at red light zone (600–700 nm) when they are excited from 220 nm to 310 nm, while emit at orange light (~ 600 nm) when excited from 310 nm to 580 nm (Fig. 3b). It is worth noting that the fluorescence of this kind of red-emitting CPDs is excitation-wavelength-independent [22, 35].
Open image in new window
a UV-Vis absorption, excitation (peak at 600 nm), and b emission (excited 220–580 nm) spectra of SA-CPDs
Two-photon photoluminescence properties of SA-CPDs before and after the powdering process are shown in Fig. 4a. There is a blue shift from 602 nm (before the powdering process) to 529 nm (after the powdering process) at the same excitation wavelength of 850 nm by femtosecond pulse laser (30 mW). The PL intensity was increased after the powdering process.
Open image in new window
Two-photon photoluminescence spectra of SA-CPDs (a) and confocal fluorescence microscopy images of HeLa cells treated with SA-CPDs excited by 850 nm, 30 mW femtosecond pulse laser (b–e)
SA-CPDs powders were re-dissolved in PBS (1X) and was applied in HeLa cells imaging using confocal fluorescence microscopy and 850 nm femtosecond pulse laser (30 mW) (see Fig. 4b–e). After cultured with HeLa cells for 12 h, SA-CPDs were swallowed by HeLa cells, and CPDs entered cytoplasm. The FL intensity of red channel (645–675 nm) is weak while the green channel (526–574 nm) is bright, it is consistent with the blue shift in the powdering process.
A facile method of acid-assisted hydrothermal route to prepare carbon dots and the application of bio-imaging were reported. Within H2SO4-, HCl- and HClO4-assisted systems, SA-CPDs prepared from H2SO4-assisted system is the brightest CPDs with the average size of ~ 5 nm, the QYs of 21.4%, and the product yield of 16.5%. SA-CPDs aqueous solution emits at 600 nm when excited by light from 300 to 580 nm. The emission wavelength is excitation-wavelength-independent. In addition, SA-CPDs have two-photon photoluminescence properties emitting at 602 nm when excited by 850 nm femtosecond pulse laser (30 mW). The method has also been utilized in imaging for HeLa cells and has the potential in, e.g., bio-imaging applications.
Funding was received from the National Natural Science Foundation of China (61405062, 61675071, 61471186, 91233208), the Guangdong Provincial Science Fund for Distinguished Young Scholars (2018B030306015), Pearl River Nova Program of Guangzhou (201710010010), Guangdong innovative Research Team Program (201001D0104799318), Guangdong Natural Science Foundation of Guangdong Province (S2013040014211, 2014A030313445), China Postdoctoral Science Foundation (2013 M530368, 2014 T70818), Guangdong Provincial Key Laboratory of Optical Information Materials and Technology (2017B030301007), Joint International Research Laboratory of Optical Information and the Key Laboratory of Optoelectronic, Devices and Systems of Ministry of Education and Guangdong Province and the Discipline and Specialty, and Construction Foundation of Colleges and Universities of Guangdong Province (2013LYM_0017).
Availability of Data and Materials
All of the original data and materials are available in different sheets of the Excel file (Additional file 2).
CT proposed the new synthesis method for red carbon dots and carried out all the experiments of chemical procession, characterization, optical spectra, and measurements. CZ carried out the experiments of cell culture and treatment. XP operated the laser equipment and confocal microscope for cell imaging. HZ carried the calculation of the formation energy of the carbon dots. DW, QZ, and SH participated in the design and coordination of this study. All authors read and approved the final manuscript.
The authors declare that they have no competing interests.
Springer Nature remains neutral with regard to jurisdictional claims in published maps and institutional affiliations.
11671_2018_2657_MOESM1_ESM.doc (1.2 mb)
Additional file 1: Figure S1. Photos of CPDs samples under UV light (365 nm). Figure S2. The optimization process for HA-CPDs preparation with HCl-assisted p-PD system. Figure S3. (a) The suitable c (p-PD) range for the preparation of red CPDs at the optimized c (acid):c (p-PD) ratio. (b) QYs data and the intensity plots as a function of absorbance for the as-prepared CPDs excited at 365 nm. Samples in (a) were excited at 365 nm. (c) Photographs of all as-prepared and diluted C-dots samples under daylight and 365 nm UV light. (d) SA-CPDs powders and (e) the re-dissolved solution. (DOC 1178 kb)
11671_2018_2657_MOESM2_ESM.xlsx (217 kb)
Additional file 2: Sheet 1. Raw data of the size distribution. Sheet 2. Raw data of FT-IR. Sheet 3. Raw data of QYs. Sheet 4. Raw data of UV-Vis absorption and excitation. Sheet 5. Raw data of emission spectra. Sheet 6. Raw data of two-photon photoluminescence spectra. (XLSX 216 kb)
Durán N, Simões MB, de Moraes ACM, Fávaro WJ, Seabra AB (2016) Nanobiotechnology of carbon dots: a review. J Biomed Nanotechnol 12(7):1323–1347CrossRefGoogle Scholar
Xu TS, Li XY, Xie ZH, Li XG, Zhang HY (2015) Poly (o-phenylenediamine) nanosphere-conjugated capture antibody immobilized on a glassy carbon electrode for electrochemical immunoassay of carcinoembryonic antigen. Microchim Acta 182(15–16):2541–2549CrossRefGoogle Scholar
Ge J, Jia Q, Liu W, Guo L, Liu Q, Lan M, Zhang H, Meng X, Wang P (2015) Red-emissive carbon dots for fluorescent, photoacoustic, and thermal theranostics in living mice. Adv Mater 27(28):4169–4177CrossRefGoogle Scholar
Bao L, Liu C, Zhang ZL, Pang DW (2015) Photoluminescence-tunable carbon nanodots: surface-state energy-gap tuning. Adv Mater 27(10):1663–1667CrossRefGoogle Scholar
Wang J, Zhang P, Huang C, Liu G, Leung KC, Wang YX (2015) High performance photoluminescent carbon dots for in vitro and in vivo bioimaging: effect of nitrogen doping ratios. Langmuir 31(29):8063–8073CrossRefGoogle Scholar
Wang D, Wang ZY, Zhan QQ, Pu Y, Wang JX, Foster NR, Dai LM (2017) Facile and scalable preparation of fluorescent carbon dots for multifunctional applications. Engineering 3(3):402–408CrossRefGoogle Scholar
Jiang K, Sun S, Zhang L, Wang Y, Cai C, Lin H (2015) Brightly yellow-emissive N-doped carbon dots: preparation, cellular imaging and bifunctional sensing. ACS Appl Mate Inter 7(41):23231CrossRefGoogle Scholar
Vedamalai M, Periasamy AP, Wang CW, Tseng YT, Ho LC, Shih CC, Chang HT (2014) Carbon nanodots prepared from o-phenylenediamine for sensing of cu(2+) ions in cells. Nanoscale 6(21):13119–13125CrossRefGoogle Scholar
Yan S, Yang SW, He L, Ye CC, Song X, Liao F (2014) Quantum size effect of poly (o-phenylenediamine) quantum dots: from controllable fabrication to tunable photoluminescence properties. Synthetic Met 198:142–149CrossRefGoogle Scholar
Lv X, Wang X, Huang D, Nie C, Zeng G, Niu Q (2014) Quantum dots and p-phenylenediamine based method for the sensitive determination of glucose. Talanta 129(21):20–25CrossRefGoogle Scholar
Feng J, Chen YL, Han YX, Liu JJ, Ren CL, Chen XG (2016) Fluorescent carbon nanoparticles: a low-temperature trypsin-assisted preparation and Fe3+ sensing. Anal Chim Acta 926:107–117CrossRefGoogle Scholar
Liu S, Qin X, Tian J, Wang L, Sun X (2012) Photochemical preparation of fluorescent 2,3-diaminophenazine nanoparticles for sensitive and selective detection of Hg (II) ions. Sensors Actuators B Chem 171-172(8):886–890CrossRefGoogle Scholar
Zhang Z, Zheng T, Li X, Xu J, Zeng H (2016) Progress of carbon quantum dots in photocatalysis applications. Part Part Syst Charact 33(8):457–472CrossRefGoogle Scholar
Hu S, Wei Z, Chang Q, Trinchi A, Yang J (2016) A facile and green method towards coal-based fluorescent carbon dots with photocatalytic activity. Appl Surf Sci 378:402–407CrossRefGoogle Scholar
Chang Q, Li KK, Hu SL, Dong YG, Yang JL (2016) Hydroxyapatite supported N-doped carbon quantum dots for visible-light photocatalysis. Mater Lett 175:44–47CrossRefGoogle Scholar
Wei W, Xu C, Wu L, Wang J, Ren J, Qu X (2014) Non-enzymatic-browning-reaction: a versatile route for production of nitrogen-doped carbon dots with tunable multicolor luminescent display. Sci Rep 4(1):3564CrossRefGoogle Scholar
Mirtchev P, Henderson EJ, Soheilnia N, Yip CM, Qzin GA (2011) Solution phase synthesis of carbon quantum dots as sensitizers for nanocrystalline TiO2 solar cells. J Mater Chem C 22(4):1265–1269CrossRefGoogle Scholar
Kwon W, Do S, Kim JH, Jeong MS, Rhee SW (2015) Control of photoluminescence of carbon nanodots via surface functionalization using para-substituted anilines. Sci Rep 5:12604CrossRefGoogle Scholar
Paulo S, Stoica G, Cambarau W, Martinez-Ferrero E, Palomares E (2016) Carbon quantum dots as new hole transport material for perovskite solar cells. Synt Met 222:17–22CrossRefGoogle Scholar
Baker SN, Baker GA (2010) Luminescent carbon nanodots: emergent nanolights. Chem Int Ed 49:6726–6744CrossRefGoogle Scholar
Zhu SJ, Song YB, Zhao XH, Shao JR, Zhang JH, Yang B (2015) The photoluminescence mechanism in carbon dots (graphene quantum dots, carbon nanodots, and polymer dots): current state and future perspective. Nano Res 8(2):355–381CrossRefGoogle Scholar
Ding CQ, Zhu AW, Yang T (2014) Functional surface engineering of C-dots for fluorescent biosensing and in vivo bioimaging. Acc Chem Res 47:20–30CrossRefGoogle Scholar
Jiang K, Sun S, Zhang L, Lu Y, Wu AG, Cai CZ, Lin HW (2015) Red, green, and blue luminescence by carbon dots: full-color emission tuning and multicolor cellular imaging. Angew Chem 54(18):5360–5363CrossRefGoogle Scholar
Ding H, Yu SB, Wei JS, Xiong HM (2016) Full-color light-emitting carbon dots with a surface-state-controlled luminescence mechanism. ACS Nano 10(1):484–491CrossRefGoogle Scholar
Tan CL, Su XY, Zhou C, Wang BJ, Zhan QQ, He SL (2017) Acid-assisted gydrothermal synthesis of red fluorescent carbon dots for sensitive detection of Fe (III). RSC Adv 7:40952–40956CrossRefGoogle Scholar
Song W, Duan WX, Liu YH, Ye ZJ, Chen YL, Chen HL, Qi SD, Wu J, Liu D, Xiao LH, Ren CL, Chen XG (2017) Ratiometric detection of intracellular lysine and pH with one-pot synthesized dual emissive carbon dots. Anal Chem 89(24):13626–13633CrossRefGoogle Scholar
Liu JJ, Li DW, Zhang K, Yang MX, Sun HC, Yang B (2018) One-step hydrothermal synthesis of nitrogen-doped conjugated carbonized polymer dots with 31% efficient red emission for in vivo imaging. Small 14:1703919CrossRefGoogle Scholar
Grabolle M, Spieles M, Lesnyak V, Gaponik N, Eychmüller A, Reschgenger U (2009) Determination of the fluorescence quantum yield of quantum dots: suitable procedures and achievable uncertainties. Anal Chem 81:6285–6294CrossRefGoogle Scholar
Frisch M, Trucks G, Schlegel H, Scuseria G, Robb M, Cheeseman J, Scalmani G, Barone V, Mennucci B, Petersson G (2009) Gaussian 09, revision A. Gaussian, Inc., WallingfordGoogle Scholar
Xing LD, Borodin O, Smith GD, Li WS (2011) Density functional theory study of the role of anions on the oxidative decomposition reaction of propylene carbonate. J Phys Chem A 115:13896–13905CrossRefGoogle Scholar
Qu S, Zhou D, Li D, Ji W, Jing P, Han D, Liu L, Zeng H, Shen D (2016) Toward efficient orange emissive carbon nanodots through conjugated sp2-domain controlling and surface charges engineering. Adv Mater 28(18):3516–3521CrossRefGoogle Scholar
Tang L, Ji R, Li X, Bai G, Liu CP, Hao J, Jiang H, Teng KS, Yang Z, Lau SP (2014) Deep ultraviolet to near-infrared emission and photoresponse in layered N-doped graphene quantum dots. ACS Nano 8:6312–6320CrossRefGoogle Scholar
Gao ZH, Lin ZZ, Chen XM, Zhong HP, Huang ZY (2016) A fluorescent probe based on N-doped carbon dots for highly sensitive detection of Hg2+ in aqueous solutions. Analy Methods 8:2297–2304CrossRefGoogle Scholar
Craciun AM, Diac A, Focsan M, Socaci C, Maqyari K, Maniu D, Mihalache I, Veca LM, Astilean S, Terec A (2016) Surface passivation of carbon nanoparticles with p-phenylenediamine towards photoluminescent carbon dots. RSC Adv 6:56944–56951CrossRefGoogle Scholar
Wang H, Sun C, Chen XQ, Zhang Y, Colvin VL, Rice Q, Seo J, Feng SY, Wang SN, Yu WW (2017) Excitation wavelength independent visible color emission of carbon dots. Nanoscale 9:1909–1915CrossRefGoogle Scholar
© The Author(s). 2018
Open AccessThis article is distributed under the terms of the Creative Commons Attribution 4.0 International License (http://creativecommons.org/licenses/by/4.0/), which permits unrestricted use, distribution, and reproduction in any medium, provided you give appropriate credit to the original author(s) and the source, provide a link to the Creative Commons license, and indicate if changes were made.
Authors and Affiliations
Chunlin Tan1View author's OrcID profileChao Zhou1Xingyun Peng1Huozhen Zhi3Dan Wang4Qiuqiang Zhan1Email authorSailing He12Email author1.Centre for Optical and Electromagnetic Research, Guangdong Provincial Key Laboratory of Optical Information Materials and Technology, South China Academy of Advanced OptoelectronicsSouth China Normal UniversityGuangzhouChina2.JORCEP, Department of Electromagnetic EngineeringRoyal Institute of TechnologyStockholmSweden3.Engineering Research Center of MTEES (Ministry of Education), School of Chemistry and EnvironmentSouth China Normal UniversityGuangzhouChina4.State Key Laboratory of Organic-Inorganic CompositesBeijing University of Chemical TechnologyBeijingChina